**Combination of theoretical analysis and FTIR to study** **the photocurrent oscillation of Silicon in fluoride media**

F. Yahyaoui^{1}, L. Hlou^{2}, M. Aggour^{1*}

**1***Département de Physique - LPMC - Faculté des Sciences, B.P 133, 14000, Kénitra – Maroc*

**1***Département de Physique - LTNPSA - Faculté des Sciences B.P 133, 14000, Kénitra – Maroc*

To deepening our knowledge of the behaviour of the silicon/electrolyte interface, a study of photocurrent oscillations on silicon in fluoride concentration cF=0.033 M is realized, and as a confirmation of the result the investigation is extrapolated to a variety of electrolyte compositions. The etch rates of anodic oxides in diluted fluoride solutions have been determined by using a new approach of the analysis of anodic current oscillations. The time dependent thickness of the anodic oxide has been measured by in-situ FTIR and can be simulated considering only the time dependent current and the etch rate.

**I. INTRODUCTION**

The electrochemistry of silicon electrodes in fluoride
media is of great interest in semiconductor processing,
especially for devices preparation, due to control of the
process by the current flux and/or the electrode
potential. It is possible to modify the surface from
rough and/or porous to smooth and vice versa under
control of the potential and electrolyte composition. A
simple change in pH may lead to atomically flat^{/1/}, as
well as rough silicon surfaces^{/2/}. The most surprising
observation of the behaviour of silicon-electrolyte
interfaces is the photocurrent oscillations, which appear
in a certain range (above ca. 3 V vs. SCE)^{/3/}of anodic
oxidation of silicon in diluted fluoride solutions. The
appearance of oscillations on n-Si requires illumination
while the phenomenon on p-Si also takes place in the
dark, independently on crystal orientation and doping
type.

This phenomenon has been studied extensively during the last decade. However, up to now, the mechanism of the anodic current oscillations is still under discussion.

Changes in surface morphology of silicon oxide^{/4-7/},
hole formation^{/5-7/}, and variation of the amount of
oxide^{/5-8/} which is explained by non uniform anodic
oxidation leading to photocurrent oscillation^{/5,6,9/}, and
passivation of the Si/SiO_{2} interface and hydrogenated
silicon surface^{/10,11/}, are accompanying the oscillatory
behaviour.. Generally, most of the earlier studies,
assumed that the oscillations in silicon/silicon
oxide/electrolyte systems to be caused by a competition
between oxide formation (connected with current flow)
and dissolution (currentless).

The thickness of the anodic oxide layer and the relation between the etch rate and the rate of oxidation are quite important for better understanding of these processes.

The measurement of the etch rate of anodic oxides during anodic current oscillations is not simple because one has to measure the change of the amount of oxide and one has to consider the superposition of the oxidation and etch rates to get information about the etch rate. The thickness of the anodic oxides changes usually around 7 nm during the anodic current oscillations.

A theoretical model which might also describe consistently the microscopical physico-chemical events in the silicon/silicon oxide/electrolyte system has not yet been attempted, due to the complicated behaviour of chemical and physical process at surfaces.

In this paper, we present an in situ infrared spectroscopy study during photocurrent oscillations at +6V in 0.033 M (pH 3.8) in combination with a theoretical approach for the dissolution and formation of an oxide layer on silicon.

**II. **

**EXPERIMENTAL**

Phosphorus-doped n-Si(111) wafers (resistivity 20-35

### Ω

cm, float-zone purified) and boron-doped p-Si(100) wafers (resistivity 5 or 200 Ωcm) served as working electrodes. For in-situ FTIR measurements, the samples were cut from a 0.5 mm thick polished wafer, shaped as 15-15 mm^{2}platelets, and 45° bevelled for use as multiple-total-internal-reflection prisms. The platelets were provided with ohmic contact using 600°C evaporation of gold-antimony alloy and indium soldering on the gold pads.

The electrochemical cell was equipped with a platinum counter-electrode, and an Ag/AgCl (in saturated KCl) reference electrode.

The electrolytes were prepared from solutions of 1M
HF, 1M N_{4}HF, and 1M NH_{4}Cl in ultra pure water^{/12/}.
The pH was adjusted by adding droplets of H_{2}SO_{4}.

40 The potential was stepped from the rest potential -0.5 V

to +6 V under illumination (in the case of photocurrent oscillations on n-Si) and from -0.4 V to +6.9 V without illumination (in the case of anodic current oscillations on p-Si). In this cases, large current oscillations are triggered.

The anodic oxide was characterized by using IR
vibrational spectroscopy in the potential difference
mode (so-called Subtractively Normalized Fourier-
Transform IR Spectroscopy- SNIFTIRS) at a BOMEM
MB100 Fourier-Transform IR spectrometer^{/13/} in the
multiple internal reflection geometry (10 reflections).

The IR electric field was parallel to the Si / electrolyte
interface (s-polarisation). The reference spectrum was
recorded for the hydrogenated silicon surface at V_{0}~
0.5 V. See for more details also Ref.^{/14/}.

**III. RESULTS AND DISCUSSION**

Figure 1 shows IR absorbance spectra during
photocurrent oscillations at minimal and maximal
thickness of the anodic oxide layer (0.033 M N_{4}HF, pH
3.8). The associated absorbance spectra contain the
typical features of the Si-O-Si vibration modes around
1100 cm^{-1} and IR absorption at 1700 cm^{-1} and between
3100 and 3500 cm^{-1} which are related to the H2O
scissor and stretching modes, respectively^{/21/}.

Figure.1: IR absorbance spectra at the maximum and at
the minimum of the thickness of the anodic oxide
during photocurrent oscillations for n-Si in 0.033 M
NH_{4}F, pH 3.8.

The oxide thickness (d_{ox}) can be calculated from the
normalised FTIR spectra (δI/I) integrated over the
region of the Si-O-Si vibration modes by using the
following equation:

(1)

where n_{1}, θ, σ, Ay and C are the refractive index of the
ATR prism (n_{i} = 3.42), the incidence angle (θ = 45°),
the wave number, a numerical coefficient taking into
account the geometry^{/19/} (A_{y} = 2.32) and a constant in
the definition of the dielectric function (C = 1500^{/20/}),
respectively.

A typical example for the time dependence of
photocurrent oscillations and of the respective
thickness of the anodic oxide is presented in figure 2
for n-Si in 0.033 M NH_{4}F (pH 3.8). The oscillations are
regular and the period is about 300 s at these
conditions. The amplitude and the frequency of the
photocurrent oscillations depend strongly on the
composition of the electrolyte and on the applied
potential^{/16/}. The thickness of the anodic oxide layer
(d_{ox}) adopts a similar oscillation behaviour as the
photocurrent, result which is already experimentally
supplied by FTIR^{/15,18/}. d_{ox} changes between 4 and 11
nm for the given electrolyte. There is a phase shift
between the photocurrent maxima and the
corresponding oxide thickness. Such phase shift has
been also reported by Aggour et al.^{/16/} and Chazalviel^{/18/}

et al. and has to do with the time dependent relation between the oxidation and etch rates.

Figure.2: Time dependence of the photocurrent
oscillations (a) and of the respective thickness of the
anodic oxide (b) for n-Si in 0.033 M NH_{4}F, pH 3.8 at U

= +6 V.

We found that the current densities at which the
maximal and minimal thickness of the anodic oxide
layers (d_{max} and d_{min}, respectively) are reached, are
identical. For this reason, a value of a current j_{M}

jM= j d( max)=j d( min) (2) can be defined independently of the concentration and of the pH of the diluted fluoride solution. As remark,

1000 2000 3000 4000

0,0 0,5

F T IR -s p e ctra d u rin g an o d ic o xid atio n
0 .0 33 M N H_{4}F , p H 3 .8

O -H

νS iO _{δ} _{ν}S iH
O H_{2}

Absorbance

W avenum ber (cm^{-1})

a t th e IR m a xim u m a t th e IR m in im u m

### ∫

### ⋅ ⋅

### ⋅

### = ⋅ δ σ

### π

### θ *d*

*I* *I* *C* *A* *d* *n*

*y*

*ox* 2

1

### cos

0 300 600 900

(b) (a) U = +6 n-Si(111), 30 Ωcm 0.033 M NH4F, pH 3.8

iPh (µA/cm²)

0 500 1000 1500

0 4 8 12

dox (nm)

Time (s)

the value of j_{M} is practically equal to the average
current density (for example, 56 and 60 µA/cm²,
respectively, for 0.033 M N_{4}HF, pH 3.8 at +6 V). For
this reason, the average current can be also used
(instead of j_{M}) in the following considerations.

The dependence of the maximal and minimal
thickness of the anodic oxide and of the difference of
both on the pH is given in figure 3 for n-Si in 0.033 M
NH_{4}F. The value of d_{max} is about 8 nm and nearly
constant for pH up to 3.0 and increases to 10-11 nm
with increasing pH (pH changed up to 4.3). At the
higher pH, d_{max} tends again to saturation. In difference
to d_{max}, the value of d_{min} decreases with increasing pH
while d_{min} tends to saturation for the lower pH and to a
decrease for pH > 4.0. As result, the difference d_{max} -
d_{min} increases continuously from about 1 nm at pH 2.5
to 7 nm at pH 4.0. The value of d_{max} - d_{min} increases
with increasing pH and therefore with decreasing etch
rate and saturates at lower etch rates. It would be
interesting to carry out experiments in the range of very
low etch rates (pH close to 5) to get more detailed
information.

Figure.3: Dependence of the maximal and minimal
thickness of the anodic oxide and of the difference of
both on the pH for n-Si in 0.033 M NH_{4}F.

The change of the oxide thickness in time is given by
the difference between the oxidation rate (K_{ox}) and the
etch rate of the anodic oxide (R):

∂

∂ dox

t =Kox −R (3)

The etch and oxidation rates are equal at d_{max} and
d_{min} (equation(2)). Oxide formation or etching
predominate when j > jM or j < jM, respectively.

The density of the anodic current at a given time t is determined by the oxidation rate

j t Kox t Q t ( ) ( ) t( )

=α =δ

δ (4)

where α and δQ(t) are a proportionality factor and the charge flown within the time interval δt. The flown charge normalized to the surface area is given by δQ(t)

= 4⋅q⋅δN(t), where q = 1.6⋅10^{-19} As and δN(t) is the
amount of oxidized Si-atoms. The factor 4 appears due
to the fact that 4 holes are consumed for the oxidation
of a Si-atom in the overall oxidation reaction^{/17/}. The
amount of oxidized Si atoms determines the thickness
of the oxide layer formed within δt (δdox(t)) and it can
be written: δN(t) = ρ⋅NA⋅δdox(t) / M (M = 60 g/mol -
molar mass of SiO_{2}, ρ = 2.2 g/cm³ - the specific gravity
of SiO_{2} and N_{A} = 6.022⋅10^{23 } /mol - Avogadros
number). Since K_{ox} = δd_{ox}) / (tδt, one will get α =
4⋅q⋅ρ⋅NA / M and therefore;

R M

q NA jM

=α^{−} =
ρ

1

j 4

M (5)

In the following, we will consider a constant etch
rate R given by equation (5) independent of time and of
d_{ox}. As remark, equation (5) corresponds in principle
only to the etch rate at times when d_{ox }= d_{min} or d_{ox} =
d_{max}. The thickness of the oxide layer at a given time
t_{i+1} (d_{ox}(t_{i+1})) is determined by the thickness of the
oxide layer at a given earlier time t_{i} (d_{ox}(t_{i})) and by the
integrated current density with respect to j_{M} which
separates the regions where etching or oxide growth
dominate (integral from t_{i} to t_{i+1}):

(6)
An initial value d_{ox}(t_{0}) can be determined by FTIR. We
point out that equation (6) implements a constant etch
rate and that for this reason equation (6) can be used to
prove this assumption by comparing the measured and
calculated values of d_{ox}. Figure 4 shows an example for
a time dependence of d_{ox}(t) (0.033 M NH_{4}F, pH 3.8, U

= 6V) for simulation after equation (6) and for
measured values. As expected, the simulated thickness
of the anodic oxide adopts a similar oscillation
behavior as the photocurrent (Fig.4a). The simulated
and measured values of d_{ox}(t) are practically equal what
gives evidence that R can be really assumed as constant
for the given experimental conditions. This fact is not
trivial since the microscopic structure of thin anodic
oxides may depend on the thickness and therefore R
would not be constant. Obviously, the thin anodic
oxide layers are quite homogenous between 4 and 12
nm. Chazalviel et al. found some evidence for a time
dependent etch rate^{/18/}. Probably, the slight deviations
between the simulated and measured values at lower
oxide thickness are caused by changes in R.

## ∫

^{+}

^{−}

### ⋅ +

### =

^{−}

+

1

### ) ) ( ( )

### ( )

### (

_{1}

^{1}

*i*

*i*

*t*

*t*

*M*
*i*

*ox*
*i*

*ox*

*t* *d* *t* *j* *t* *j* *dt*

*d* α

2 3 4

0 5 10

n-Si(111), 30 Ωcm
0.033 M NH_{4}F

d_{max}
d_{min}
d_{max}-d_{min}

Measured oxide thickness (nm)

pH

42 A phase shift has been observed between the simulated

and measured time dependencies of d_{ox} (see figure 4,
the measured values are slightly retarded). This shows
that the model of equation (6) is to simple for the exact
description of d_{ox}(t). For example, rates of transport
through the thin anodic oxide layer should be taken into
account for more sophisticated models.

Figure.4: Time dependence of the photocurrent
oscillations (a) and of the respective measured (circles)
and simulated (line) thickness of the anodic oxide (b)
for n-Si in 0.033 M NH_{4}F, pH 3.8 at U = +6 V.

Equation (5) allows the experimental determination of the etch rate of anodic oxide as well as the oxidation rate (for the pH and the molarity considered) by measuring the time dependent anodic current. Eq.5 is valid not only for the photocurrent oscillations of n-Si also for the anodic current oscillations of p-Si.

Usually, HF and HF_{2}^{-} are considered to etch silicon
oxides according to the following reaction equations:

SiO_{2} + 6 HF → SiF62- + H_{2}O + 2 H^{+} (7a)
SiO_{2} + 3 HF_{2}^{-}→ SiF62- + H_{2}O + OH^{- }

(7b)

The crucial importance of the pH of the solution for the
etching of silicon oxides was demonstrated in earlier
experiments^{/22,23/}. The influence of the pH on the
chemical equilibrium in the electrolyte and therefore on
the concentrations of the [HF] and [HF2-

] components
is evident^{/24/}:

k_{1}[HF] = [H^{+}] [F^{-}] with k_{1 }= 1.3 x 10^{-3} mol/l (8a)
k_{2}[HF_{2}^{-}] = [HF] [F^{-}] with k_{2 }= 0.104 mol/l

(8b)

The total concentration of fluor in the electrolyte (c_{F}) is
given by;

c_{F} = 2[HF_{2}^{-}] + [HF] + [F^{-}]
(9)

At low pH values (between 2 and 5), the etching occurs
mainly by HF_{2}^{-}, but it becomes negligible for pH values
exceeding 5.

Attempts have been made to separate the different
reaction mechanisms, but none of the attempts so far
have yielded a model which was valid for the whole
range of HF concentrations. In fact, especially for the
low concentrations, Judge^{/25/} was the first who
proposed a qualitative description of the dissolution
rate of a thermal oxide, based on two reactive species,
HF_{2}^{−}and HF, where the former act four to fives times
faster then the later one:

R = a [HF] + b [HF_{2}^{-}] + c
(10)

where a and b contain activation energy-type terms (at
25°C: a= 0.25, b= 0.97, and c=-0.014^{/25/} if the unit of R
is nm/s).

In the aim to extract the etch rate of the anodic oxide,
we achieve values of J_{M} from the photocurrent
oscillations measured in c_{F} = 0.033 M at different pH
values (from pH 2.5 to pH 4.3). The data points shown
in figure 5, acquired from Eq. 5 for 0.033M (open
circle), have been fitted by Judge model in a wide pH
range from 0 to 7(solid line). With the given
coefficients (above) Judge’s formulae fails to adjust our
acquired points from Eq.5, but it succeeded to improve
the adaptation of our points with various coefficients. A
good fitting (dashed line) is succeeded with:

a=5.385±0.368, b=33.361±10.867, and c=-0.013±0.007 From this fitting, we see that the coefficient b can be determined only with large standard error, but the value

of c is almost in accordance with that given by Judge.

To test the validity of the determined coefficients, the obtained fitting parameters will then be used to adjust the etch rate calculated as well as for the concentration 0.05M by using the Eq.5.

0 200 400

(b) (a)

n-S i(111),
0.033 M N H_{4}F, pH 3.8
U = +6 V

i (µA/cm²)

1200 1400 1600

4 6 8 10

12 m easurem ent

sim ulation

Time (s) dox (nm)

0 1 2 3 4 5 6 7

0,0 0,1 0,2 0,3 0,4

R calculated from eq.5 for 0.033M Judge simulation (0.033M) Judge simulation with different coefficients R calculated from eq.5 for 0.05M Created curve for 0.05M with 0.033M's coefficients R fitted for 0.05M with again coefficients

Etch rate (nm/s)

pH

Figure 5: The etch rate calculated from Eq.5, for 0.033M(open circle), its curve- fitting by judge formulae with the given coefficients(solid circle), and with the found one (solid), the etch rate (from Eq.5) for 0.05M (diamond), with the found coefficients for 0.033M(dashed), and with another’s coefficients(doted) as function of pH.

As can be seen from Fig. 5, if we keep the same coefficients found for 0.033M fixed, the adaptation for 0.05M (solid circle) exceeds all the data points(diamond). An almost good fit is obtained as when the fitting(doted) is done with;

a=7.870±0.284, b=28.103±5.883, and c= -0.022±0.009.

Consequently judge model fails in our conditions, thus one needs to change the coefficients in passing from a concentration to the other.

Later, Kikuyama et .al^{/26/}, found that etching of SiO_{2} by
HF2− occurs according to the following relationship
with R(HF_{2}^{−}) in nm/s;

R= a HF_{2}^{−} +b HF_{2}^{−} log( H^{+} / HF_{2}^{−} ) (11)
With a and b are two parameters dependent on the
report of [H^{+}] and [HF_{2}^{−}] as;

a= 2.138, b=0.648. when ( H^{+} / HF_{2}^{−} ) ≥ 2.10^{-2}.
They determined this relation in modified buffered HF
at pH values ≥ 2. This shows that in the etching
reaction of HF_{2}^{−} with SiO_{2}, H^{+} also play a role.

In our case H^{+} / HF_{2}^{−} ratio is always larger than 1,
since;

H^{+} + NH^{+}4 = F^{−} + HF2^{−} + OH^{−} + cl^{−} (12)
due to the charge neutrality.

Figure 6, shows the adjustment of the etch rate R calculated from Eq.5 with the formula proposed by kikuyama (Eq.11).

Fig. 6: The etch rate calculated from Eq.5(open circle),
its curve- fitting by judge(solid), by Kikuyama with the
given coefficients(cross), and the found coefficients
(square) as function of pH, for c_{F }= 0.033M

This model also not succeeded to adjust our points by considering the coefficients given by Kikuyama(doted line). In the object to try to perfect the adaptation by kikuyama’s formulae, again coefficients are found by itteratif calculation,

a= 287.496 ± 25.261 and b= 47.210 ± 6.105 (square).

For Kikuyama model, the mechanism of why the H^{+}
ion concentration influence SiO2 etching is changed at
the H^{+} / HF_{2}^{−} ratio of 2.10^{-2} was not justified, also
from Eq.11 the etching rate depends mainly on the
HF_{2}^{−} concentration which is clear for pH superior to
2.5, on the other hand the Kikuyama’s model does not
involve any contribution from HF, however it is
necessary to take it into account, especially if pH < 2.5.

In order to improve these formulae (Eqs.10 and 11), and optimize the conditions of parameters, from experimental points access to a more general expression of R in a large pH range [0-7] may be taken.

For this fact, being based on formulae proposed by
Judge^{/25/} and the study of the others authors/26/, we
have deduced that this multitude of formulae take
account only a development of R in first order of
concentration. None of these equation has given the
good concordance with the obtained results, especially
for pH larger than 2, in which the etching occurs
mainly by the HF_{2}^{−}.

However, we tried to find a formula which can satisfy our results by combination of Judge's model (Eq. 10) and that of Kikuyama (Eq.11), we found that the etch rate can best be described by the following equation;

R =c_{F}( (a H F + HF_{2}^{−} )+b HF_{2}^{−} log ( H^{+} / HF_{2}^{−} ))
(13)

As can be seen, Eq.13 is a second-order equation in
concentration, the dependence of the etching rate both
of [HF] and HF_{2}^{−} concentrations is taking into
account. The H^{+} also play a role in the etching rate, but
the functionality of

### [H

^{+}

### ]

is small, because it changes logarithmically. This relation (Eq.13) is valid for solutions where theThe calculation of R from the above relationship (Eq.13) has given the curve-fitting (solid) in Fig. 7, with adjustment parameters a and b given with their errors;

a =158.843 ± 5.207, b = 93.193 ± 15.962.

0,00 0,02 0,04 0,06 0,08 0,10 0,12 0,14 0,16 0,18

R calculated from eq.5 for 0.033M Judge's simulation with the news coefficients Kikuyama'simulation with the news coefficients Kikuyama'simulation with the given coefficients

Etch rate / nm.s-1

44 The standard error on the coefficients is low, which

means that the accuracy of the coefficients obtained is high.

therefore the given formulae have succeeded to have a good concordance.

Figure. 7: The etch rate from Eq.5 (open circle), its
curve- fitting by Eq.13 (solid) as function of pH, for c_{F}

= 0.033M

Furthermore, from Fig.4 if the current density
undergoes a little change relatively to J_{M}, consequently
also a local pH variation will take place. One can
explain this such as, when oxide formation
predominates, the current increases and therefore the
pH decreases, whereas it increases when currentless
etching prevails.

Since the etch rate depends on pH of the electrolyte, the etching process is therefore accelerated in the time range of highest current and delayed for low current densities.

Fig. 8: The etch rate from Eq.5 (solid symbols), and its
curve- fitting (solid) as function of pH, for c_{F }= 0.05
M, c_{F }= 0.1 M, and c_{F }= 0.2 M.

To supplement our investigations, aiming to confirm
the validity of our model, we also extended it to other
concentrations namely; c_{F} = 0.05 M, c_{F} = 0.1 M and 0.2
M, the points data of the etch rate are calculated from
the measured average photocurrent by Eq.5, and then
fitted with the above relationship (Eq.13).

For each concentration c_{F}, R as well as its curve-fitting
are presented as a function of the pH in Fig. 8.

The fit is established for the same values of a and b
obtained for c_{F} = 0.033 M. They are in good agreement
with the experimental results.

Then we conclude that knowing the fluoride
concentration c_{F}, and the pH of the used electrolyte, the
etch rate can be determined by the equation presented
above (Eq.13). Which is ascertained at least for the
used electrolyte in this work.

**VI**

**. Conclusion**

Our study reveal that knowing the used electrolyte composition, one can anticipate the magnitudes and variations of some parameters, such as photocurrent, oxide thickness. A new approach for the determination of the etch rates and oxidation rates of thin anodic layers has been proposed on the basis of correlation between anodic current oscillations and the anodic oxide thickness in diluted fluoride solutions.

The time dependent thickness can be well simulated by taking into account only the time dependent anodic current oscillations and a constant etch rate.

**Acknowledgement**

The authors are grateful to Professor J.-N. Chazalviel and F. Ozanam, LPMC- Ecole Polytechnique, for IR- spectroscopy measurements.

**References**

[1]: G. S. Higashi, Y. J. Chabal, G. W. Trucks and K.

Raghavachari, Appl. Phys. Lett., 56 (1990) 656.

[2]: V. A. Burrows, Y. J. Chabal, G. S. Higashi, K.

Raghavachari and S. B. Christman, Appl. Phys. Lett., 53 (1988) 998.

[3]: D. R. Turner, J. Electrochem Soc., 105(1958) 402.

[4]: J. Rappich, H. Jungblut, M. Aggour, and H.-J.

Lewerenz, , J. Electrochem. Soc. 141, L99 (1999).

[5]: H.-J. Lewerenz, M. Aggour, J. Electroanal. Chem.

351, 159-168 (1993)

[6]: M. Aggour, M. Giersig and H.-J. Lewerenz, J.

Electroanal. Chem. 383, 67 (1995).

[7]: J. Rappich, M. Aggour, S. Rauscher, H. Jungblut, and H.-J. Lewerenz, Surf. Sci. 335, 160(1995).

[8]: O. Nast, S. Rauscher, H. Jungblut, and H.-J.

Lewerenz, J. Electroanal. Chem. 422, 169-174(1998) [9]: F. Ozanam, and J.-N. Chazalviel, J. Electron Spectrosc. Relat. Phenom. 64/65, 395 (1993).

[10]: J. Rappich, V. Y. Timoshenko, R.Würz, and T.

Dittrich, Electrochim. Acta, , (2000).

[11]: S. Rauscher, T. Dittrich, M. Aggour, J. Rappich and H.-J. Lewerenz, Appl. Phys. Lett. 66, 3018 (1995).

0 1 2 3 4 5 6 7

0,00 0,02 0,04 0,06 0,08 0,10 0,12 0,14 0,16 0,18 0,20

pH

Etch rate / nm.s-1

Eq.5 Eq.13

2,0 2,5 3,0 3,5 4,0 ^{0}

50 100 150 200 250

pH JM /µA.cm-2

0 1 2 3 4 5 6 7

0 1 2 3 4 5 6 7

Calculated etch rate / nm.s-1

pH

R from eq.5 for cF=0.05M R from eq.5 forcF=0.1M R from eq.5 forcF=0.2M R from eq.13

[12]: Hamdy. H. Hassan, PHD Thesis, University of Ain Shams, Egypt (1994).

[13]: F. Ozanam, and J.-N. Chazalviel, Rev.Sci. Inst., 59(1988) 242.

[14]: C. da Fonseca, F. Ozanam, J.-N. Chazalviel, Surf.

Sci 365 (1996) 1-14

[15]: H.-J. Lewerenz, J. Phys. Chem. B (1997), 101, 2421-2425

[16]: F. Ozanam, J.-N. Chazalviel, A. Radi and M.

Etman, Ber. Bunsenges. Phys. Chem. 95 (1991) 98.

[17]: E. Duffek, E. Benjamini, and C. Mylroie, Electrochem. Technol. 3, 75 (1965)

[18]: J.-N. Chazalviel, C. da Fonseca, and F. Ozanam, J. Electrochem. Soc., 145 (1998) 964-973.

[19]: Y. Chabal, Surf. Sci. Rep., 8, 211(1988).

[20]: C. T. Kirk, Phys. Rev. B, 38, 1255 (1988) [21]: Y. J. Chabal, S. B. Christman, Phys. Rev. B 29, 6974 (1984).

[22]: H.-J. Lewerenz, Electrochim. Acta, 37, 847(1992).

[23]: J. Stumper and H.-J. Lewerenz, J. Electroanal.

Chem. Interfacial Electrochem., 274, 11 (1989)

[24]: R. E. Mesmer and C. F. Baes, Inorg. Chem. 8, 618 (1969)

[25]: J. S Judge, J. Electrochem. Soc., 118(1971)1772.

[26]: H. Kikuyama, N. Miki, K. Saka, J. Takano, I.

kawanabe, M. Miyashita and t. Ohmi, IEEE Trans.

Semiconductor Manufacturing, Vol. 4, No.1, Feb.

(1991).